- Nano Express
- Open Access
Paclitaxel-incorporated nanoparticles using block copolymers composed of poly(ethylene glycol)/poly(3-hydroxyoctanoate)
© Kim et al.; licensee Springer. 2014
- Received: 21 August 2014
- Accepted: 20 September 2014
- Published: 24 September 2014
Block copolymers composed of poly(3-hydroxyoctanoate) (PHO) and methoxy poly(ethylene glycol) (PEG) were synthesized to prepare paclitaxel-incorporated nanoparticle for antitumor drug delivery. In a 1H-NMR study, chemical structures of PHO/PEG block copolymers were confirmed and their molecular weight (M.W.) was analyzed with gel permeation chromatography (GPC). Paclitaxel as a model anticancer drug was incorporated into the nanoparticles of PHO/PEG block copolymer. They have spherical shapes and their particle sizes were less than 100 nm. In a 1H-NMR study in D2O, specific peaks of PEG solely appeared while peaks of PHO disappeared, indicating that nanoparticles have core-shell structures. The higher M.W. of PEG decreased loading efficiency and particle size. The higher drug feeding increased drug contents and average size of nanoparticles. In the drug release study, the higher M.W. of PEG block induced the acceleration of drug release rate. The increase in drug contents induced the slow release rate of drug. In an antitumor activity study in vitro, paclitaxel nanoparticles have practically similar anti-proliferation activity against HCT116 human colon carcinoma cells. In an in vivo animal study using HCT116 colon carcinoma cell-bearing mice, paclitaxel nanoparticles have enhanced antitumor activity compared to paclitaxel itself. Therefore, paclitaxel-incorporated nanoparticles of PHO/PEG block copolymer are a promising vehicle for antitumor drug delivery.
- Block copolymer
- Drug delivery
Nanoparticles have been extensively investigated in the biomedical field as a drug delivery vehicle due to their properties such as small particle size less than 1,000 nm, favorable biodistribution, and drug targeting possibility [1, 2]. Among them, core-shell type nanoparticles have great potentials in the antitumor drug delivery system since they have intrinsic properties, i.e., hydrophobic core as a drug reservoir and hydrophilic outershell as a protective layer [2, 3]. They have superior properties such as extended blood circulation time of drug, passive targeting of solid tumor, dissolution of hydrophobic drugs, and enhanced biodegradation.
Poly(3-hydroxyoctanoate) (PHO) is one of the polyesters derived from bacterial source [4, 5]. PHO has attractive properties as a biomedical material such as low melting temperature and crystallinity and excellent elastomeric and mechanical properties compared to other kinds of polyhydroxyalkanoates [4–6]. The drawback of PHO is slower degradation rate and higher hydrophobic properties than other kinds of PHAs . Therefore, various chemical modifications of PHO have been attempted to endow hydrophilic properties and to improve mechanical properties as a biomedical material [5, 7].
In this study, we synthesized block copolymers composed of PHO/PEG to make core-shell-typed nanoparticles and to fabricate suitable vehicles for antitumor drug delivery. Since PHO has hydrophobicity, it could be consisted in the core of the nanoparticles while PEG must be hydrated to the direction of aqueous environment. Paclitaxel was selected as an anticancer agent due to its poor aqueous solubility. Characteristics of nanoparticles of PHO/PEG block copolymers were analyzed and antitumor activity of drug-incorporated nanoparticles was studied in vitro/in vivo.
PHO was produced by Pseudomonas oleovorans ATCC 29347 (American Type Culture Collection (ATCC), Manassas, VA 20110, USA) as reported previously  and purified from the lyophilized cells by extraction with hot chloroform . The purified PHO analyzed by gas chromatography was consisted of 7% 3-hydroxyhexanoate and 93% 3-hydroxyoctanoate. Methoxy poly(ethylene glycol)-amine (molecular weight (M.W.) = 2,000, 5,000, 12,000 g/mol) was purchased from Sunbio Co. Ltd., Cheonan, Korea. Fluorescein isothiocyanate (FITC), N,N′-dicyclohexyl carbodiimide (DCC), and N-hydroxysuccinimide (NHS) were purchased from Aldrich Chemical Company (St Louis, MO, USA). The dialysis membranes with molecular weight cut-offs (MWCOs) of 12,000 and 8000 g/mol were purchased from Spectra/PorTM dialysis membrane (Spectrum Laboratories Inc, Rancho Dominguez, CA, USA). Dichloromethane (DCM), dimethylformamide (DMF), tetrahydrofuran (THF), methanol, and acetone were of extra pure grade.
Synthesis of PHO/PEG block copolymers
Characterization of PHO/PEG block copolymer
Characterization of the synthesized polymers was performed in CDCl3 by 500 mHz 1H-NMR spectroscopy (500 mHz superconducting FT-NMR spectrometer, Varian Unity Inova 500 MHz NB High Resolution FT NMR; Varian Inc, Santa Clara, CA, USA). Molecular weight of polymers was measured with the gel permeation chromatography (GPC) system (Waters 2690D-2410, Waters, MA, USA) as described previously . GPC was equipped with a Waters 6000 solvent delivery system, RI detector, and a Rheodyne injector. Phenogel columns of 500, 103, 104, and 105 Å were used. A standard curve was established with standard polystyrene samples.
Preparation of paclitaxel-incorporated nanoparticles using PHO/PEG block copoylmer
PHO/PEG block copolymer was dissolved in 5 ml of THF and then paclitaxel dissolved in 2 ml of DMF was added. This solution was slowly dropped into 10 ml of cold deionized water for 15 min and then stirred magnetically for 60 min at 4°C. After that, this solution was dialyzed using a dialysis tube (MWCO = 12,000 g/mol) against deionized water for 1 day. To remove solvent, deionized water was exchanged at every 2-h intervals. After that, dialyzed solution was used for analysis or lyophilization. Empty nanoparticles were prepared in the absence of paclitaxel.
Drug content and loading efficiency were measured using a UV-1201 spectrophotometer (Shimadzu Co. Ltd., Kyoto, Japan) at 273 nm. Empty nanoparticles were used as a blank.
Morphology of the polymeric micelles was observed using a transmission electron microscope (TEM, JEOL JEM-2000 FX II, JEOL, Akishima-shi, Japan). One drop of nanoparticle solution containing phosphotungstic acid 0.05% (w/w) was placed onto a carbon film coated on a copper grid for TEM. Observation was done at 80 kV. The particle size of the nanoparticles was measured with dynamic laser scattering (DLS-7000, Otsuka Electronics Company, Osaka, Japan).
Drug release study
The release experiment was carried out in vitro as follows: Paclitaxel-incorporated nanoparticle solution was prepared as described above. After the dialysis procedure, the volume of nanoparticle solution was adjusted to 50 ml and then 5 ml of this solution was introduced into a dialysis tube (MWCO = 12,000 g/mol) and then dialysis tube was introduced into a 200-ml bottle with 95 ml of phosphate-buffered saline (PBS, 0.1 M, pH 7.4, 0.1% (w/v) Tween 80). This bottle was placed in a shaking incubator with stirring speed of 100 rpm at 37°C. At specific time intervals, the media were taken for analysis of drug concentration. After that, the whole media was replaced with fresh PBS to prevent drug saturation. The concentration of the paclitaxel released into PBS was evaluated using a high-performance liquid chromatography (HPLC, PerkinElmer, Waltham, MA, USA) using Phenomenex Sphereclone 5 micro ODS(2) 250 mm × 4.6 mm column and 75% methanol as a moving phase. The Flexar HPLC system (PerkinElmer, Waltham, MA, USA) was equipped with a Solvent Manager 5-CH degasser, an autosampler, a quaternary LC pump, a column oven, and a UV-visible detector. The flow rate was set to 1.5 ml/min and the temperature at 50°C. The UV detector (226 nm) was used for the measurement. To prepare the sample for the measurement of HPLC, paclitaxel was dissolved in ethanol, making 20 μl for injection.
Antitumor activity of paclitaxel-incorporated nanoparticles in vitro
Antitumor activity of paclitaxel-incorporated nanoparticles was evaluated using HuCC-T1 human cholangiocarcinoma cells. HCT116 cells were seeded at a density of 2 × 103 cells per well in 96-well plates with 100 μl of RPMI1640 supplemented with 10% FBS and incubated overnight at 37°C and 5% CO2 atmosphere. After that, free paclitaxel, paclitaxel-incorporated nanoparticles and empty nanoparticles were added to 96-well plates at 100 μl. For paclitaxel treatment, paclitaxel dissolved in DMSO was diluted 1,000 times with RPMI1640 supplemented with 10% FBS and added to cells. For nanoparticle treatment, paclitaxel-incorporated nanoparticles were diluted with RPMI1640 supplemented with 10% FBS and treated to cells. Controls were treated with 0.1% v/v of dimethyl sulfoxide. For the testing of cellular cytotoxicity of empty nanoparticles, they were diluted with serum-free RPMI1640 media and sterilized with a 0.8-μm syringe filter and added to 2 × 104 HCT116 cells. Viable cells were evaluated with MTT cell proliferation assay as described previously . After 3 days of incubation, 30 μl of MTT (5 mg/ml) was added to the 96-well plates and incubated for 4 h. The formazan crystals formed were solubilized with SDS solution (100 μl of SDS-HCl solution (SDS 10% w/v, 0.01 M HCl)) and the absorbance (560-nm test/630-nm reference) was determined using an automated computer-linked microplate reader (Infinite M200 Pro microplate reader, Molecular Device Company, Sunnyvale, CA, USA). Each measurement of drug concentration was obtained as the mean value of eight wells. The amount of formazan present is proportional to the number of viable cells, because only living cells will reduce MTT to blue formazan. The results were expressed as a percentage of the absorbance present in the drug-treated cells compared with that in the control cells.
Apoptosis and necrosis of HCT116 cells were analyzed by flow cytometry . FITC-annexin V and PI were employed to analyze apoptosis and necrosis of HCT116 cells, respectively. Cells (1 × 106 cells) were exposed to paclitaxel or paclitaxel-incorporated nanoparticles in serum-free RPMI1640 media for 48 h, and cells were washed with phosphate-buffered saline (PBS). The cells were harvested by trypsinization, and cell pellets were resuspended in a binding buffer (pH 7.4, 10 mM HEPES, 150 mM NaCl, 5 mM KCl, 1 mM MgCl2, 1.8 mM CaCl2) containing FITC-annexin V (1 μg/ml) and then further incubated for 30 min. Ten minutes prior to termination of incubation, PI (10 μg/ml) were added to stain necrotic cells under dark conditions. Following that, the cells were immediately analyzed using a FACScan flow cytometer (Becton Dicknson Biosciences, San Jose, CA, USA).
Antitumor activity of paclitaxel-incorporated nanoparticles against animal tumor xenograft
The tumor xenograft model was employed to assess antitumor activity of paclitaxel or paclitaxel-incorporated PA nanoparticles. HCT116 cells (5 × 106) were implanted subcutaneously in the backs of mice (Athymic nude BALB/c male mice, 20 g). When the diameter of tumor mass was approximately 2 ~ 3 mm (10 days after), paclitaxel or paclitaxel-incorporated nanoparticles were injected intravenously via tail vein of the mouse (paclitaxel dose = 10 mg/kg). The treatment group was divided as follows; control - 200 μl of PBS (0.01 M, pH 7.4); paclitaxel treatment - paclitaxel dissolved in Cremophor® EL/ethyl alcohol (5:5, (v/v)) solution were mixed with aqueous solution of empty nanoparticles; paclitaxel-nanoparticles prepared from PHO/PEG 5 K - lyophilized nanoparticles were reconstituted in deionized water and sterilized with a 0.8-μm syringe filter. Five mice were used for each treatment group. At intervals of 5 days, length and width of solid tumor was measured and tumor volume was calculated with the following equation: Tumo volume (mm3) = Length × Width2. Tumor mass was taken from the back of mice and the weight of tumor was compared between each of the treatment groups 2.5 weeks after drug injection. All animal experiments followed the guidelines of the Committee for the Care and Use of Laboratory Animals of Pusan National University.
Results of animal experiments were expressed as average ± standard deviation, and statistical significance was evaluated using the Student's t test (SigmaPlot program version 11.2, Systat software, Inc., CA 95110, USA). A p value <0.05 was considered significant.
Characterization of PHO/PEG block copolymer
Characterization of PHO/PEG block copolymers
M.W. of PEG (g/mol)a
M.W. by GPC (g/mol)
Particle size (weight average, nm)
PHO/PEG 2 K
PHO/PEG 5 K
PHO/PEG 12 K
Characterization of paclitaxel-incorporated nanoparticles
Characterization of paclitaxel-incorporated nanoparticles of PHO/PEG block copolymer
Drug contents (%, w/ w)
Particle size (weight average, nm)
PHO/PEG 2 K
PHO/PEG 5 K-1
PHO/PEG 5 K-2
PHO/PEG 12 K
Antitumor activity of paclitaxel-incorporated nanoparticles
Nanoparticles are regarded as ideal vehicles for anticancer drug targeting due to their intrinsic physicochemical properties . Even though various active targeting using receptor-ligand interaction strategy have been investigated successively [12–15], passive targeting using plain nanoparticles or PEGylated nanoparticles are still preferentially considered for tumor targeting due to the vasculature permeability of tumor tissue [16, 17]. Bae insisted that numerous biological and physiological elimination mechanisms of tumor preferentially decide the fate of nanovehicles prior to their access in the tumor cells . Until the nanocarriers are close to the cell surfaces, no specific interaction between receptor on the tumor cell surface and ligand on the nanoparticle surface happens. At this moment, the preferential translocation of nanoparticles from blood circulation to tumor vasculature (so-called enhanced permeation and retention (EPR) effect) is still considered for a solid tumor targeting [16, 17]. Diameter of nanoparticles less than 200 nm are known to have advantages for drug targeting because this size could increase blood circulation by avoiding reticuloendothelial system (RES) and then increase chance to access the microvessel of the tumor tissue [17, 18].
In this study, we synthesized PHO/PEG block copolymers and prepared paclitaxel-incorporated core-shell-typed nanoparticles for anticancer drug delivery. There are very few reports on the drug delivery application with PHO in spite of their defined structure and good biocompatibility [6, 19–21]. The main drawback of PHO is slow degradation in vitro and in vivo[6, 19]. In a previous research, graft-copolymerization with PEG accelerated hydrolytic degradation of polymers . PHO/PEG block copolymer was synthesized by the attachment of PEG to the carboxylic end of PHO. We prepared PHO/PEG block copolymers by varying M.W. of PEGs and its effect on the physicochemical properties of nanoparticle formation. We found that higher M.W. of PEG decreased particle size of nanoparticles even though it slightly decreased drug loading contents (in Tables 1 and 2).
For antitumor drug delivery, paclitaxel was selected as an anticancer drug because it is commonly used in the clinics and has strong hydrophobic property (aqueous solubility is less than 0.3 μg/ml) and it has a specific interaction with serum proteins . Due to its poor aqueous solubility, specific surfactant/solvent mixtures (Cremophor EL/ethanol mixture) are commercially used. However, due to the intrinsic toxicity of specific surfactant, various formulations for enhancing aqueous solubility of paclitaxel have been investigated such as nanoparticles, liposomes, and polymeric micelles . Since PEG has a protective effect for the adsorption of protein and macrophage cells, PEGylation of nanocarriers may enhance blood circulation time of nanocarriers, unwanted content with serum protein/macrophage cells, and then chance to contact tumor tissues in vivo.
Paclitaxel was incorporated into the nanoparticles by nanoprecipitation and dialysis procedure. The size of paclitaxel nanoparticles was slightly increased compared to that of empty nanoparticles. Even though the diameter of nanoparticles was increased with paclitaxel loading, the average size of nanoparticles did not exceed 200 nm. Furthermore, paclitaxel was slowly released from the nanoparticles for over 6 days. In a drug release study, diffusion from nanoparticles must be the preferential mechanism rather than the degradation of polymer because PHO itself has very slow degradation kinetics [6, 19]. Nanoparticles showed practically similar anticancer activity against tumor cells as shown in Figure 4. Furthermore, nanoparticles showed practically similar effect on the apoptosis and necrosis of tumor cells as shown in Figure 5. Antitumor activity of paclitaxel nanoparticles in vivo was evaluated using HCT116 tumor-bearing mice as shown in Figure 6. As shown in Figure 6, paclitaxel nanoparticles significantly inhibited growth of tumor mass compared to the control and the paclitaxel plus empty nanoparticles. Even though nanoparticles have no practical advantages in anticancer activity in vitro, they properly suppressed growth of tumor mass in vivo the tumor xenograft model as shown in Figure 6 while paclitaxel itself seemed to have minimal anticancer activity. The EPR effect of the nanoparticles can be considered to explain these results, i.e., nanoparticles properly entered into the cells and killed the tumor cells [16, 17]. Otherwise, paclitaxel itself could be absorbed to the serum protein in the blood and rapidly cleared from blood circulation. Then, these factors can induce decrease in opportunities for tumor targeting . Therefore, paclitaxel nanoparticles formed by PHO/PEG block copolymer are a promising vehicle for antitumor drug delivery.
Paclitaxel-incorporated nanoparticles were prepared using PHO/PEG block copolymers for antitumor drug delivery. Paclitaxel-incorporated nanoparticles of PHO/PEG block copolymer have spherical morphology with small particle size less than 100 nm. In a 1H-NMR study in D2O, the core-shell structure of PHO/PEG nanoparticles was confirmed. The higher M.W. of PEG decreased loading efficiency of drug and particle size. The higher drug feeding resulted in increased drug contents and average size of nanoparticles. The higher M.W. of PEG block accelerated drug release rate while higher drug contents delayed the release rate of drug. In an antitumor activity study using HuCCT1 cells in vitro, paclitaxel-incorporated nanoparticles have similar antiproliferation activity against HCT116 tumor cells. However, paclitaxel nanoparticles showed enhanced antitumor activity against HCT116 tumor cells of mice in vivo.
This study was supported by the Research Institute for Convergence of Biomedical Science and Technology (30-2014-009), Pusan National University, Yangsan Hospital.
- Kreuter J: Drug targeting with nanoparticles. Eur J Drug Metab Pharmacokinet 1994, 19: 253–256. 10.1007/BF03188928View ArticleGoogle Scholar
- Gref R, Minamitake Y, Peracchia MT, Trubetskoy V, Torchilin V, Langer R: Biodegradable long-circulating polymeric nanospheres. Science 1994, 263: 1600–1603. 10.1126/science.8128245View ArticleGoogle Scholar
- Jeong YI, Cheon JB, Kim SH, Nah JW, Lee YM, Sung YK, Akaike T, Cho CS: Clonazepam release from core-shell type nanoparticles in vitro. J Control Release 1998, 51: 169–178. 10.1016/S0168-3659(97)00163-6View ArticleGoogle Scholar
- Kim DY, Kim YB, Rhee YH: Evaluation of various carbon substrates for the biosynthesis of polyhydroxyalkanoates bearing functional groups by Pseudomonas putida. Int J Biol Macromol 2000, 28: 23–29. 10.1016/S0141-8130(00)00150-1View ArticleGoogle Scholar
- Kim HW, Chung CW, Rhee YH: UV-induced graft copolymerization of monoacrylate-poly(ethylene glycol) onto poly(3-hydroxyoctanoate) to reduce protein adsorption and platelet adhesion. Int J Biol Macromol 2005, 35: 47–53. 10.1016/j.ijbiomac.2004.11.007View ArticleGoogle Scholar
- Kim HW, Chung CW, Hwang SJ, Rhee YH: Drug release from and hydrolytic degradation of a poly(ethylene glycol) grafted poly(3-hydroxyoctanoate). Int J Biol Macromol 2005, 36: 84–89. 10.1016/j.ijbiomac.2005.03.016View ArticleGoogle Scholar
- Arkin AH, Hazer B, Borcakli M: Chlorination of poly(3-hydroxy alkanoates) containing unsaturated side chains. Macromolecules 2000, 33: 3219–3223. 10.1021/ma991535jView ArticleGoogle Scholar
- Kim DY, Jung SB, Choi GG, Kim YB, Rhee YH: Biosynthesis of polyhydroxyalkanoate copolyester containing cyclohexyl groups by Pseudomonas oleovorans. Int J Biol Macromol 2001, 29: 145–150. 10.1016/S0141-8130(01)00144-1View ArticleGoogle Scholar
- Jeong YI, Kim DH, Chung CW, Yoo JJ, Choi KH, Kim CH, Ha SH, Kang DH: Doxorubicin-incorporated polymeric micelles composed of dextran-b-poly(DL-lactide-co-glycolide) copolymer. Int J Nanomedicine 2011, 6: 1415–1427.View ArticleGoogle Scholar
- Xiao RZ, Zeng ZW, Zhou GL, Wang JJ, Li FZ, Wang AM: Recent advances in PEG-PLA block copolymer nanoparticles. Int J Nanomedicine 2010, 5: 1057–1065.Google Scholar
- Leroux JC, Allemann E, Jaeghere FD, Doelker E, Gurny R: Biodegradable nanoparticles – from sustained release formulations to improved site specific drug delivery. J Control Release 1996, 39: 339–350. 10.1016/0168-3659(95)00164-6View ArticleGoogle Scholar
- Egusquiaguirre SP, Igartua M, Hernández RM, Pedraz JL: Nanoparticle delivery systems for cancer therapy: advances in clinical and preclinical research. Clin Transl Oncol 2012, 14: 83–93. 10.1007/s12094-012-0766-6View ArticleGoogle Scholar
- Basile L, Pignatello R, Passirani C: Active targeting strategies for anticancer drug nanocarriers. Curr Drug Deliv 2012, 9: 255–268. 10.2174/156720112800389089View ArticleGoogle Scholar
- Ambasta RK, Sharma A, Kumar P: Nanoparticle mediated targeting of VEGFR and cancer stem cells for cancer therapy. Vasc Cell 2011, 3: 26. 10.1186/2045-824X-3-26View ArticleGoogle Scholar
- Choi KY, Saravanakumar G, Park JH, Park K: Hyaluronic acid-based nanocarriers for intracellular targeting: interfacial interactions with proteins in cancer. Colloids Surf B Biointerfaces 2012, 99: 82–94.View ArticleGoogle Scholar
- Bae YH: Interview with Dr You Han Bae: ligand-mediated versus ‘passive’ targeting approaches in nanoparticle oncology research. Ther Deliv 2012, 3: 933–936. 10.4155/tde.12.62View ArticleGoogle Scholar
- Danquah MK, Zhang XA, Mahato RI: Extravasation of polymeric nanomedicines across tumor vasculature. Adv Drug Deliv Rev 2011, 63: 623–639. 10.1016/j.addr.2010.11.005View ArticleGoogle Scholar
- Kwon G, Suwa S, Yokoyama M, Okano T, Sakurai Y, Kataoka K: Enhanced tumor accumulation and prolonged circulation times of micelle-forming poly (ethylene oxide-aspartate) block copolymer-adriamycin conjugates. J Control Release 1994, 29: 17–23. 10.1016/0168-3659(94)90118-XView ArticleGoogle Scholar
- Marois Y, Zhang Z, Vert M, Beaulieu L, Lenz RW, Guidoin R: In vivo biocompatibility and degradation studies of polyhydroxyoctanoate in the rat: a new sealant for the polyester arterial prosthesis. Tissue Eng 1999, 5: 369–386. 10.1089/ten.1999.5.369View ArticleGoogle Scholar
- Babinot J, Guigner JM, Renard E, Langlois V: A micellization study of medium chain length poly(3-hydroxyalkanoate)-based amphiphilic diblock copolymers. J Colloid Interface Sci 2012, 375: 88–93. 10.1016/j.jcis.2012.02.042View ArticleGoogle Scholar
- Zhang C, Zhao L, Dong Y, Zhang X, Lin J, Chen Z: Folate-mediated poly(3-hydroxybutyrate-co-3-hydroxyoctanoate) nanoparticles for targeting drug delivery. Eur J Pharm Biopharm 2010, 76: 10–16. 10.1016/j.ejpb.2010.05.005View ArticleGoogle Scholar
- Otagiri M: Study on binding of drug to serum protein. Yakugaku Zasshi 2009, 129: 413–425. 10.1248/yakushi.129.413View ArticleGoogle Scholar
- Singla AK, Garg A, Aggarwal D: Paclitaxel and its formulations. Int J Pharm 2002, 235: 179–192. 10.1016/S0378-5173(01)00986-3View ArticleGoogle Scholar
This article is published under license to BioMed Central Ltd. This is an Open Access article distributed under the terms of the Creative Commons Attribution License (http://creativecommons.org/licenses/by/4.0), which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly credited.